#------------------------------------------------------------------------------
#$Date: 2025-11-29 21:38:25 +0100 (Sat 29 de Nov de 2025) $
#$Revision: 303766 $
#$URL: svn://www.crystallography.net/cod/cif/7/71/94/7719433.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7719433
loop_
_publ_author_name
'Ridley, Christopher J.'
'Abdeldaim, Aly H.'
'Bull, Craig L.'
'Tustain, Katherine'
'Clark, Lucy'
_publ_section_title
;
 Pressure-induced tuning of the triangular-honeycomb structure of
 ferroelectric quantum spin liquid candidate, TbInO₃.
;
_journal_issue                   42
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              15696
_journal_page_last               15700
_journal_paper_doi               10.1039/d5dt01863c
_journal_volume                  54
_journal_year                    2025
_chemical_formula_moiety         'In O3 Tb'
_chemical_formula_structural     'In O3 Tb'
_chemical_formula_sum            'In O3 Tb'
_chemical_formula_weight         321.747
_chemical_name_common            'Terbium indium oxide'
_space_group_crystal_system      hexagonal
_space_group_IT_number           185
_space_group_name_Hall           'P 6c -2'
_space_group_name_H-M_alt        'P 63 c m'
_symmetry_space_group_name_H-M   'P 63 c m'
_audit_update_record
;
2025-07-19 deposited with the CCDC.	2025-09-10 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   6.2660(3)
_cell_length_b                   6.2660(3)
_cell_length_c                   12.2284(11)
_cell_measurement_pressure       3.86742
_cell_measurement_temperature    293.00000
_cell_volume                     415.80(5)
_diffrn_ambient_temperature      293.00000
_diffrn_detector                 'ZnS scintillator'
_diffrn_detector_type            custom
_diffrn_measurement_device_type  'PEARL diffractometer'
_diffrn_radiation_monochromator  none
_diffrn_radiation_type           Neutron
_diffrn_source                   'Pulsed neutron source'
_diffrn_source_target            W
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details
;
Calculated using MANTID routines.
;
_exptl_crystal_density_diffrn    7.70960
_pd_instr_dist_spec/detc         800
_pd_instr_dist_src/spec          12800
_pd_instr_location               'SNS, Oak Ridge National Lab'
_pd_meas_2theta_fixed            90
_pd_meas_scan_method
;
Time-of-flight
;
_pd_proc_info_data_reduction
;
Data reduction performed using Mantid
;
_pd_proc_info_excluded_regions
;
?
;
_pd_proc_ls_background_function  'Chebychev polynomial'
_pd_proc_ls_pref_orient_corr
;
No requirement for preferred orientation correction
;
_pd_proc_ls_prof_R_factor        3.32386
_pd_proc_ls_prof_wR_expected     2.00311
_pd_proc_ls_prof_wR_factor       4.08115
_pd_spec_mounting                'TiZr Capsule'
_pd_spec_mount_mode              transmission
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   2.03741
_refine_ls_matrix_type           sparse
_refine_ls_number_parameters     43
_refine_ls_R_I_factor            3.09680
_refine_ls_shift/su_max          0.0066
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            d5dt01863c1.cif
_cod_data_source_block           p13
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_space_group_crystal_system' value 'Hexagonal' was changed
to 'hexagonal' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 8170 2020-07-09 18:12:32Z antanas 

 Adding full bibliography for 7719421--7719440.cif.
;
_cod_original_cell_volume        415.79(5)
_cod_original_formula_sum        'In O3 Tb '
_cod_database_code               7719433
_pr_proc_ls_profile_function
;
Voigt function convoluted with a back-to-back double exponential.
;
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, -y, z+1/2 '
'-x+y, -x, z '
'-x+y, y, z+1/2 '
'-y, -x, z+1/2 '
'-y, x-y, z '
'y, -x+y, z+1/2 '
'y, x, z '
'x-y, -y, z '
'x-y, x, z+1/2 '
'-x, -x+y, z '
'x, x-y, z+1/2 '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_symmetry_multiplicity
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Tb1 Tb 2 0 0 0.267(3) 1 0.1
Tb2 Tb 4 0.3333333 0.6666667 0.237(3) 1 0.1
In1 In 6 0.345(4) 0 0 1 0.1176497
O1 O 6 0.308(2) 0 0.1637(18) 1 0.3151487
O2 O 6 0.654(3) 0 0.3234(19) 1 0.3151487
O3 O 2 0 0 0.477(3) 1 0.3151487
O4 O 4 0.3333333 0.6666667 0.027(2) 1 0.3151487
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
O2 Tb1 O2 111.2(9) 1_455 1_555 6_545
O2 Tb1 O2 111.2(9) 3_665 1_555 1_455
O2 Tb1 O2 111.2(9) 3_665 1_555 6_545
O1 Tb1 O2 76.6(5) 1_555 1_555 3_665
O1 Tb1 O2 164.6(17) 1_555 1_555 1_455
O1 Tb1 O2 76.6(5) 1_555 1_555 6_545
O1 Tb1 O1 93.0(12) 6_555 1_555 1_555
O1 Tb1 O2 76.6(5) 6_555 1_555 3_665
O1 Tb1 O2 76.6(5) 6_555 1_555 1_455
O1 Tb1 O2 164.6(17) 6_555 1_555 6_545
O1 Tb1 O1 93.0(12) 3_555 1_555 6_555
O1 Tb1 O1 93.0(12) 3_555 1_555 1_555
O1 Tb1 O2 164.6(17) 3_555 1_555 3_665
O1 Tb1 O2 76.6(5) 3_555 1_555 1_455
O1 Tb1 O2 76.6(5) 3_555 1_555 6_545
O3 Tb1 O1 123.1(9) 1_555 1_555 3_555
O3 Tb1 O1 123.1(9) 1_555 1_555 6_555
O3 Tb1 O1 123.1(9) 1_555 1_555 1_555
O3 Tb1 O2 72.3(10) 1_555 1_555 3_665
O3 Tb1 O2 72.3(10) 1_555 1_555 1_455
O3 Tb1 O2 72.3(10) 1_555 1_555 6_545
O2 Tb2 O2 100.5(11) 6_555 1_555 3_665
O2 Tb2 O2 100.5(11) 1_565 1_555 6_555
O2 Tb2 O2 100.5(11) 1_565 1_555 3_665
O1 Tb2 O2 75.1(6) 3_665 1_555 1_565
O1 Tb2 O2 174.7(13) 3_665 1_555 6_555
O1 Tb2 O2 77.6(5) 3_665 1_555 3_665
O1 Tb2 O1 106.5(10) 1_565 1_555 3_665
O1 Tb2 O2 77.6(5) 1_565 1_555 1_565
O1 Tb2 O2 75.1(6) 1_565 1_555 6_555
O1 Tb2 O2 174.7(13) 1_565 1_555 3_665
O1 Tb2 O1 106.5(10) 6_555 1_555 1_565
O1 Tb2 O1 106.5(10) 6_555 1_555 3_665
O1 Tb2 O2 174.7(13) 6_555 1_555 1_565
O1 Tb2 O2 77.6(5) 6_555 1_555 6_555
O1 Tb2 O2 75.1(6) 6_555 1_555 3_665
O4 Tb2 O1 67.7(9) 1_555 1_555 6_555
O4 Tb2 O1 67.7(9) 1_555 1_555 1_565
O4 Tb2 O1 67.7(9) 1_555 1_555 3_665
O4 Tb2 O2 117.4(9) 1_555 1_555 1_565
O4 Tb2 O2 117.4(9) 1_555 1_555 6_555
O4 Tb2 O2 117.4(9) 1_555 1_555 3_665
O4 In1 O1 83.9(8) 1_545 1_555 1_555
O4 In1 O4 120.7(13) 8_555 1_555 1_545
O4 In1 O1 83.9(8) 8_555 1_555 1_555
O2 In1 O4 99.1(8) 2_654 1_555 8_555
O2 In1 O4 99.1(8) 2_654 1_555 1_545
O2 In1 O1 173.7(15) 2_654 1_555 1_555
O3 In1 O2 82.8(13) 2_554 1_555 2_654
O3 In1 O4 119.0(7) 2_554 1_555 8_555
O3 In1 O4 119.0(7) 2_554 1_555 1_545
O3 In1 O1 90.9(13) 2_554 1_555 1_555
Tb1 O1 In1 129.7(13) 1_555 1_555 1_555
Tb2 O1 Tb1 102.8(9) 1_545 1_555 1_555
Tb2 O1 In1 108.5(10) 1_545 1_555 1_555
Tb2 O1 Tb2 100.8(9) 8_555 1_555 1_545
Tb2 O1 Tb1 102.8(9) 8_555 1_555 1_555
Tb2 O1 In1 108.5(10) 8_555 1_555 1_555
O4 O1 Tb2 59.8(8) 8_555 1_555 8_555
O4 O1 Tb2 120.9(7) 8_555 1_555 1_545
O4 O1 Tb1 134.5(4) 8_555 1_555 1_555
O4 O1 In1 49.1(7) 8_555 1_555 1_555
O4 O1 O4 82.7(8) 1_545 1_555 8_555
O4 O1 Tb2 120.9(7) 1_545 1_555 8_555
O4 O1 Tb2 59.8(8) 1_545 1_555 1_545
O4 O1 Tb1 134.5(4) 1_545 1_555 1_555
O4 O1 In1 49.1(7) 1_545 1_555 1_555
O2 O1 O4 96.4(5) 6_545 1_555 1_545
O2 O1 O4 170.6(7) 6_545 1_555 8_555
O2 O1 Tb2 113.7(11) 6_545 1_555 8_555
O2 O1 Tb2 51.8(6) 6_545 1_555 1_545
O2 O1 Tb1 51.3(6) 6_545 1_555 1_555
O2 O1 In1 135.8(6) 6_545 1_555 1_555
O2 O1 O2 82.9(10) 3_665 1_555 6_545
O2 O1 O4 170.6(7) 3_665 1_555 1_545
O2 O1 O4 96.4(5) 3_665 1_555 8_555
O2 O1 Tb2 51.8(6) 3_665 1_555 8_555
O2 O1 Tb2 113.7(11) 3_665 1_555 1_545
O2 O1 Tb1 51.3(6) 3_665 1_555 1_555
O2 O1 In1 135.8(6) 3_665 1_555 1_555
O2 O1 O2 76.1(7) 1_555 1_555 3_665
O2 O1 O2 76.1(7) 1_555 1_555 6_545
O2 O1 O4 94.6(6) 1_555 1_555 1_545
O2 O1 O4 94.6(6) 1_555 1_555 8_555
O2 O1 Tb2 50.6(5) 1_555 1_555 8_555
O2 O1 Tb2 50.6(5) 1_555 1_555 1_545
O2 O1 Tb1 104.8(11) 1_555 1_555 1_555
O2 O1 In1 125.4(10) 1_555 1_555 1_555
O3 O1 O2 172.2(10) 2_554 1_555 1_555
O3 O1 O2 109.5(6) 2_554 1_555 3_665
O3 O1 O2 109.5(6) 2_554 1_555 6_545
O3 O1 O4 79.5(7) 2_554 1_555 1_545
O3 O1 O4 79.5(7) 2_554 1_555 8_555
O3 O1 Tb2 128.3(7) 2_554 1_555 8_555
O3 O1 Tb2 128.3(7) 2_554 1_555 1_545
O3 O1 Tb1 83.0(10) 2_554 1_555 1_555
O3 O1 In1 46.7(10) 2_554 1_555 1_555
Tb1 O2 In1 107.4(14) 1_655 1_555 2_655
Tb2 O2 Tb1 104.9(9) 8_555 1_555 1_655
Tb2 O2 In1 117.5(10) 8_555 1_555 2_655
Tb2 O2 Tb2 103.2(12) 1_545 1_555 8_555
Tb2 O2 Tb1 104.9(9) 1_545 1_555 1_655
Tb2 O2 In1 117.5(10) 1_545 1_555 2_655
O1 O2 Tb2 108.8(11) 6_655 1_555 1_545
O1 O2 Tb2 53.1(6) 6_655 1_555 8_555
O1 O2 Tb1 52.1(7) 6_655 1_555 1_655
O1 O2 In1 133.3(7) 6_655 1_555 2_655
O1 O2 O1 72.1(8) 3_655 1_555 6_655
O1 O2 Tb2 53.1(6) 3_655 1_555 1_545
O1 O2 Tb2 108.8(11) 3_655 1_555 8_555
O1 O2 Tb1 52.1(7) 3_655 1_555 1_655
O1 O2 In1 133.3(7) 3_655 1_555 2_655
O3 O2 O1 97.4(7) 1_655 1_555 3_655
O3 O2 O1 97.4(7) 1_655 1_555 6_655
O3 O2 Tb2 128.1(5) 1_655 1_555 1_545
O3 O2 Tb2 128.1(5) 1_655 1_555 8_555
O3 O2 Tb1 58.5(11) 1_655 1_555 1_655
O3 O2 In1 48.9(10) 1_655 1_555 2_655
O1 O2 O3 178.8(8) 1_555 1_555 1_655
O1 O2 O1 81.7(8) 1_555 1_555 3_655
O1 O2 O1 81.7(8) 1_555 1_555 6_655
O1 O2 Tb2 51.8(6) 1_555 1_555 1_545
O1 O2 Tb2 51.8(6) 1_555 1_555 8_555
O1 O2 Tb1 120.3(13) 1_555 1_555 1_655
O1 O2 In1 132.3(11) 1_555 1_555 2_655
In1 O3 In1 118.3(4) 2_555 1_555 5_555
In1 O3 In1 118.3(4) 10_555 1_555 2_555
In1 O3 In1 118.3(4) 10_555 1_555 5_555
Tb1 O3 In1 97.5(10) 1_555 1_555 10_555
Tb1 O3 In1 97.5(10) 1_555 1_555 2_555
Tb1 O3 In1 97.5(10) 1_555 1_555 5_555
O2 O3 Tb1 49.2(7) 3_665 1_555 1_555
O2 O3 In1 48.3(6) 3_665 1_555 10_555
O2 O3 In1 117.4(9) 3_665 1_555 2_555
O2 O3 In1 117.4(9) 3_665 1_555 5_555
O2 O3 O2 81.9(11) 6_545 1_555 3_665
O2 O3 Tb1 49.2(7) 6_545 1_555 1_555
O2 O3 In1 117.4(9) 6_545 1_555 10_555
O2 O3 In1 117.4(9) 6_545 1_555 2_555
O2 O3 In1 48.3(6) 6_545 1_555 5_555
O2 O3 O2 81.9(11) 1_455 1_555 6_545
O2 O3 O2 81.9(11) 1_455 1_555 3_665
O2 O3 Tb1 49.2(7) 1_455 1_555 1_555
O2 O3 In1 117.4(9) 1_455 1_555 10_555
O2 O3 In1 48.3(6) 1_455 1_555 2_555
O2 O3 In1 117.4(9) 1_455 1_555 5_555
O1 O3 O2 138.0(3) 5_555 1_555 1_455
O1 O3 O2 90.7(6) 5_555 1_555 6_545
O1 O3 O2 138.0(3) 5_555 1_555 3_665
O1 O3 Tb1 139.9(6) 5_555 1_555 1_555
O1 O3 In1 102.7(11) 5_555 1_555 10_555
O1 O3 In1 102.7(11) 5_555 1_555 2_555
O1 O3 In1 42.3(6) 5_555 1_555 5_555
O1 O3 O1 67.9(9) 2_555 1_555 5_555
O1 O3 O2 90.7(6) 2_555 1_555 1_455
O1 O3 O2 138.0(3) 2_555 1_555 6_545
O1 O3 O2 138.0(3) 2_555 1_555 3_665
O1 O3 Tb1 139.9(6) 2_555 1_555 1_555
O1 O3 In1 102.7(11) 2_555 1_555 10_555
O1 O3 In1 42.3(6) 2_555 1_555 2_555
O1 O3 In1 102.7(11) 2_555 1_555 5_555
O1 O3 O1 67.9(9) 10_555 1_555 2_555
O1 O3 O1 67.9(9) 10_555 1_555 5_555
O1 O3 O2 138.0(3) 10_555 1_555 1_455
O1 O3 O2 138.0(3) 10_555 1_555 6_545
O1 O3 O2 90.7(6) 10_555 1_555 3_665
O1 O3 Tb1 139.9(6) 10_555 1_555 1_555
O1 O3 In1 42.3(6) 10_555 1_555 10_555
O1 O3 In1 102.7(11) 10_555 1_555 2_555
O1 O3 In1 102.7(11) 10_555 1_555 5_555
In1 O4 In1 117.5(4) 1_565 1_555 3_665
In1 O4 In1 117.5(4) 6_555 1_555 1_565
In1 O4 In1 117.5(4) 6_555 1_555 3_665
Tb2 O4 In1 99.3(7) 1_555 1_555 6_555
Tb2 O4 In1 99.3(7) 1_555 1_555 1_565
Tb2 O4 In1 99.3(7) 1_555 1_555 3_665
O1 O4 Tb2 52.5(6) 6_555 1_555 1_555
O1 O4 In1 47.0(5) 6_555 1_555 6_555
O1 O4 In1 123.5(8) 6_555 1_555 1_565
O1 O4 In1 115.1(7) 6_555 1_555 3_665
O1 O4 O1 86.8(9) 1_565 1_555 6_555
O1 O4 Tb2 52.5(6) 1_565 1_555 1_555
O1 O4 In1 115.1(7) 1_565 1_555 6_555
O1 O4 In1 47.0(5) 1_565 1_555 1_565
O1 O4 In1 123.5(8) 1_565 1_555 3_665
O1 O4 O1 86.8(9) 3_665 1_555 1_565
O1 O4 O1 86.8(9) 3_665 1_555 6_555
O1 O4 Tb2 52.5(6) 3_665 1_555 1_555
O1 O4 In1 123.5(8) 3_665 1_555 6_555
O1 O4 In1 115.1(7) 3_665 1_555 1_565
O1 O4 In1 47.0(5) 3_665 1_555 3_665
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
Tb1 O2 2.28(2) 1_555 6_545
Tb1 O2 2.28(2) 1_555 1_455
Tb1 O2 2.28(2) 1_555 3_665
Tb1 O1 2.30(3) 1_555 1_555
Tb1 O1 2.30(3) 1_555 6_555
Tb1 O1 2.30(3) 1_555 3_555
Tb1 O3 2.57(5) 1_555 1_555
Tb2 O2 2.308(19) 1_555 3_665
Tb2 O2 2.308(19) 1_555 6_555
Tb2 O2 2.308(19) 1_555 1_565
Tb2 O1 2.348(16) 1_555 3_665
Tb2 O1 2.348(16) 1_555 1_565
Tb2 O1 2.348(16) 1_555 6_555
Tb2 O4 2.56(4) 1_555 1_555
In1 O1 2.02(2) 1_555 1_555
In1 O4 2.081(12) 1_555 1_545
In1 O4 2.081(12) 1_555 8_555
In1 O2 2.16(2) 1_555 2_654
In1 O3 2.18(3) 1_555 2_554
O1 In1 2.02(2) 1_555 1_555
O1 Tb1 2.30(3) 1_555 1_555
O1 Tb2 2.348(16) 1_555 1_545
O1 Tb2 2.348(16) 1_555 8_555
O1 O4 2.74(2) 1_555 8_555
O1 O4 2.74(2) 1_555 1_545
O1 O2 2.84(2) 1_555 6_545
O1 O2 2.84(2) 1_555 3_665
O1 O2 2.92(3) 1_555 1_555
O1 O3 2.99(4) 1_555 2_554
O2 In1 2.16(2) 1_555 2_655
O2 Tb1 2.28(2) 1_555 1_655
O2 Tb2 2.308(19) 1_555 8_555
O2 Tb2 2.308(19) 1_555 1_545
O2 O1 2.84(2) 1_555 6_655
O2 O1 2.84(2) 1_555 3_655
O2 O3 2.87(3) 1_555 1_655
O2 O1 2.92(3) 1_555 1_555
O3 In1 2.18(3) 1_555 5_555
O3 In1 2.18(3) 1_555 2_555
O3 In1 2.18(3) 1_555 10_555
O3 Tb1 2.57(5) 1_555 1_555
O3 O2 2.87(3) 1_555 3_665
O3 O2 2.87(3) 1_555 6_545
O3 O2 2.87(3) 1_555 1_455
O3 O1 2.99(4) 1_555 5_555
O3 O1 2.99(4) 1_555 2_555
O3 O1 2.99(4) 1_555 10_555
O4 In1 2.081(12) 1_555 3_665
O4 In1 2.081(12) 1_555 1_565
O4 In1 2.081(12) 1_555 6_555
O4 Tb2 2.56(4) 1_555 1_555
O4 O1 2.74(2) 1_555 6_555
O4 O1 2.74(2) 1_555 1_565
O4 O1 2.74(2) 1_555 3_665
